Synthesis, Structure, Thermoelectric Properties, and Band Gaps of Alkali Metal Containing Type I Clathrates: A8Ga8Si38(A = K, Rb, Cs) and K8Al8Si38
Sui, Fan; He, Hua; Bobev, Svilen; Zhao, Jing; Osterloh, Frank E.; Kauzlarich, Susan M.; Chemistry of Materials 27 (2015) 2812–; doi:10.1021/cm504436v

data_4002197
_publ_section_title
;
 Synthesis, Structure, Thermoelectric Properties, and Band Gaps of Alkali
 Metal Containing Type I Clathrates: A8Ga8Si38(A = K, Rb, Cs) and
 K8Al8Si38
;
_journal_issue                   8
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2812
_journal_paper_doi               10.1021/cm504436v
_journal_volume                  27
_journal_year                    2015
_chemical_formula_sum            'Cs8 Ga7.8 Si38.2'
_chemical_formula_weight         2680.13
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           223
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   10.5339(3)
_cell_length_b                   10.5339(3)
_cell_length_c                   10.5339(3)
_cell_measurement_reflns_used    1003
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      27.07
_cell_measurement_theta_min      3.87
_cell_volume                     1168.87(6)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0432
_diffrn_reflns_av_sigmaI/netI    0.0102
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            9915
_diffrn_reflns_theta_full        28.26
_diffrn_reflns_theta_max         28.26
_diffrn_reflns_theta_min         2.73
_exptl_absorpt_coefficient_mu    11.563
_exptl_absorpt_correction_T_max  0.4657
_exptl_absorpt_correction_T_min  0.3970
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.807
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       bar
_exptl_crystal_F_000             1217
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.462
_refine_diff_density_min         -0.391
_refine_diff_density_rms         0.086
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.183
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_reflns         287
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.183
_refine_ls_R_factor_all          0.0149
_refine_ls_R_factor_gt           0.0127
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0151P)^2^+0.4558P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0298
_refine_ls_wR_factor_ref         0.0300
_reflns_number_gt                263
_reflns_number_total             287
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm504436v_si_004.cif
_cod_data_source_block           sad
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 

 Adding full bibliography for 4002196--4002198.cif.
;
_cod_original_sg_symbol_H-M      Pm-3n
_cod_original_formula_sum        'Cs8 Ga7.80 Si38.20'
_cod_database_code               4002197